The Effect of Sandblasting and Coating of Zirconia by Nano Composites on Bond
Strength of Zirconia to Resin Cements
Parisa Karami Zarandi, DDS 1; Azamsadat Madani, DDS 2; Hosein Bagheri, PhD 2; Maryam Moslemion, DDS 1 1
Dept. of Prosthodontics, Faculty of Dentistry, Zanjan University of Medical Science, Zanjan, Iran. 2
Dental Material Research Center, Mashhad University of Medical Science, Mashhad, Iran.
Received: November 2018; Revised: April 2019; Accepted: June 2019;
Statement of the Problem: Despite yttria-stabilized tetragonal zirconia polycrystal (Y-TZP)
high strength in dental restoration application, Zr- the framework has a low tendency to react
chemically with cement which is the main reason of these restoration failures.
Purpose: The aim of this in vitro study was to evaluate the effect of Y-TZP coating by
nano-composite of silica and aluminosilicate according to the sol-gel dip-coating technique on the
bond strength of resin cement to Y-TZP.
Materials and Method: In this experimental study, Y-TZP blocks (10×10×3 ) were
pre-pared and sintered and assigned into 4 groups (n=10) for coating including control group
with-out any further surface treatment, sandblasted using 110 μm alumina particles under 2.5 bar
and tip distance of 10 mm, silica sol dip coating + calcination, aluminosilicate sol dip coating+
calcinations. To confirm chemical bonds of sol-gel covers, Fourier transforms infrared
spec-troscopy (FT-IR) technique was used. The surface of the sample was investigated by scanning
electron microscopy (SEM), energy-dispersive spectroscopy detector (EDS) and x-ray
diffrac-tion (XRD) methods. Micro-shear bond strengths (µSBS) of zirconia-cement specimens were
evaluated. Data were analyzed with a one-way ANOVA test in SPSS version 11.5 software
with a confidence interval of 95%.
Results: µSBS of sandblasting, nano-silica, and nano-aluminosilicate specimens were
signifi-cantly higher than control. µSBS of nano-silica was higher than other groups but no significant
difference was observed in µSBS of sandblasting nano-silica, and nano-aluminosilicate groups
Conclusion: Covering the zirconia surface with non-invasive silica and
nano-aluminosilicate using the sol-gel technique leads to improved cement bond strength.
Corresponding Author: Karami P, Dept. of Prosthodontics, Faculty of Dentistry, Zanjan University of Medical Sciences, 4645ghete, 11 Sharghi, Faze 2, Shahrake Karmandan, Zanjan, Iran. Tel: +98-2433445427
Cite this article as: Karami Zarandi P, Madani A, Bagheri H, Moslemion M. The Effect of Sandblasting and Coating of Zirconia by Nano Composites on Bond Strength of Zirconia to
Resin Cements. J Dent Shiraz Univ Med Sci. March 2020; 21(1):63-68.
Surface preparation of zirconia-based dental restoration
for resin bonding is still being considered as a major
challenge. Unlike feldspathic porcelain and
glass-ceramics, zirconia cannot be etched by hydrofluoric acid
because its structure is completely made of crystalline
phase and no glassy matrix exists. Therefore, a method
other than acid etching must be used to provide
micro-structures for creating micromechanical adhesion or
chemical bonding to improve the zirconia-resin
bond-ing. So far, many researchers have examined different
methods for creating zirconia surface roughness and
improving zirconia-resin bonding [1-5]. Various
meth-ods were introduced including; application of phosphate
monomers (MDP), special primers, formulation of new
silane, applying low fusing porcelain, slurry zirconia
and silica coating [6-12]. Different methods have been
developed for silica coating on the zirconia surface,
including silica pyrolytic coating, tribochemical
coat-ing, and plasma spraying techniques, Silano-Pen
treat-ment, vapor-phase deposition, and coating using sol-gel
Table 1: Materials composition
Material Specification of material Manufacture
DD Bio ZW iso zirconoxid Yttria-stabilized tetragonal zirconia polycrystal (ZrO2+HfO2+Y203>99%)
Dental Direkt GmbH, Germany
Clearfil TM SA luting Dual cure resin cement (MDP, silane, silica and initiators) Kuraray co., Okayama, Japan Clearfil SE bond primer Methacryloxydecyl dihydrogen phosphate, ethanol Kuraray co., Okayama, Japan
Clearfil porcelain bond activator Hydrophobic aromatic dimethacrylate, 3Methacryloxypropyl
trimethoxysilane Kuraray co., Okayama, Japan
Aluminum nitrate nonahydrate Isopropanol
(C₂H₅O) ₄Si Al(NO3)3 · 9H2O CH₃CH(OH)CH₃
Merck, Germany Sigma-Aldrich, USA Merck, Germany
According to reports on silica coating techniques,
tribochemical is preferred due to improved bonding and
ease of application. In the tribochemical coating
tech-nique, the bonding surface is air-abraded with
silica-coated alumina particles. Aluminum oxide particles
sprinkled with silica are buried on the ceramic surface
by air pressure leading to a more chemically reactive
surface to the resin. This method not only provides the
silica surface for silanization but also causes
microme-chanical retention. However, literature shows that
sand-blasting with silica-coated alumina particles causes
stress on yttria-stabilized tetragonal zirconia polycrystal
(Y-TZP) due to a decrease in degradation temperature
of zirconia while the tetragonal phase transforms to
monoclinic form [21-26]. In our previous study, we
have reported the sol-gel dip coating method as a gentle,
while the effective procedure for the formation of
sili-cate and aluminosilisili-cate thin films directly from the
solution on the dental zirconia substrate to improve the
bond strength of zirconia to the porcelain. To evaluate
the coating characterization, Fourier transforms infrared
spectroscopy (FT-IR), x-ray diffraction(XRD),
scan-ning electron microscopy (SEM) and energy-dispersive
spectroscopy detector (EDS) tests were used. The
analy-sis of these tests confirmed the creation of a smooth and
uniform layer of nanocomposite on the zirconia surface
that improved the mechanical feature of the
zirconia-porcelain bond after zirconia-porcelain firing . In this study,
silica and aluminosilicate have been used through the
dip coating sol-gel method for zirconia coating to
im-prove the bond strength of zirconia to resin cement. The
null hypothesis tested was that the coating of Y-TZP
surface functionalization by different coatings has no
effect on the resin-zirconia bond strength.
Materials and Method Specimen preparation
Forty Y-TZP blocks (10×10×3 ) were prepared (D
D Bio ZW iso Zirconoxid; Dental Direkt GmbH) and
sintered as instructed by the manufacturer. The sintered
blocks were assigned into 4 groups (n=10) for
subse-quent coating including the control group without any
further surface treatment, sandblasted using 110μm
alumina particles under 2.5 bar and tip distance of
10mm, silica sol dip coating+calcination and
alumino-silicate sol dip coating+calcinations. The compositions
and manufacturers of materials used in this study are
listed in Table 1. To provide a clean surface before
coat-ing, the blocks were washed under running distilled
water, placed in an acetone/ethanol ultrasonic bath
(Elmasonic S 300 H) for 20 minutes, and then air-dried
at 70°C in Chamber Furnace - ELF11/6 .
The silica sol was prepared as described previously
. Tetraethylorthosilicate (TEOS) was added to nitric
acid (HNO3) (≥65%, Sigma-Aldrich Co.) and ethanol
(EtOH) 99.8% (Merck & Co., Inc) solution drop by
drop. After 10 minutes of deionized water (DDW) was
added to the solution, the obtained sol was stirred
vigor-ously for 1hour. The molar ratio of EtOH:HNO3:EtOH:
H2O was 1:1.7:6:2. Nano alumina-silica sol by Cao
method  was prepared. Briefly, 67 ml of TEOS was
dissolved in 100ml isopropanol. This solution was
add-ed dropwise to water and nitric acid at room
tempera-ture. This sol was stirred for 1hour. 7.36g aluminum
nitrate nonahydrate, which was dissolved in 50ml
de-ionized water, was added to partially hydrolyzed silica
sol. This sol was stirred for 12hours.
Coating of Y-TZP blocks
The Y-TZP blocks were coated by the sol using a
dip-coating device and calcinated at 400°C (5°C/min) for 2
hours. The upward and downward motion speed was 80
mm/s and the dipping time was 60 seconds . S-EM,
EDS, XRD and FTIR tests were accomplished to survey
were expressed in our previous study .
FT-IR, XRD, SEM and EDS were used to characterize
the coating and the nature of the bonding between the
coating and zirconia. The methods of these tests which
we used in this study described in our previous article
Micro-shear- bond strength testing
To evaluate the efficacy of bonding between Y-TZP and
resin cement µSBS testing was used. The coupling
agent and primer (Clearfil, Kuraray) were thoroughly
mixed according to the manufacturer instructions and
applied on the Y-TZP block with a special brush. After
placement, the whole surface was gently dried with oil-
and water-free air spray.The resin cement pastes
(Clear-fil TM, SA, Kuraray, Japan) were mixed in a weight
ratio of 1/1 and placed inside the Tygon tube with an
internal diameter of 0.8mm and a height of 2mm. The
Tygon tube was filled with cement and placed on the
block, which was applied by coupling agent and primer.
Then the excess cement was removed and the surface
was exposed to LED curing light (Elipar II, 3M ESPE
St. Paul, USA) in all directions by 1000 mW/cm2
inten-sity and 430-480 wavelength, for 40 seconds and stored
in distilled water for 24 hours. The µSBS was tested
with a universal testing machine instrument (STM20,
SANTAM, Iran) with a crosshead speed of 1mm/ min
(Figure 1). The statistical results were analyzed using
the one-way ANOVA test, which was followed by Tuk-ey's post hoc pairwise comparison (α=0.05) using SPSS V11.5 software.
The results of the analysis of the FT-IR, XRD, SEM,
and EDS tests are explained in our previous study .
The results of the µSBS test for each study group are
shown in Figure 2. Statistical analysis revealed that
there were significant differences between the study
groups. The highest µSBS is observed for silica sol dip
coated group (21.66±4.32MPa) respectively and
mini-mum bonding strength was observed in the control
group (10.63±3.48MPa). Tukey HSD post-hoc test
showed a significant difference in the control group
(10.63±3.48MPa) and other groups. There was no
sig-nificant difference between other groups (sandblasted:
18.25±2.54MPa, aluminosilicate: 17.98±6.99MPa, sili
Figure 1: Universal testing machine instrument
Figure 2: Mean value and standard deviation for µSBS exper-iment (Note:Abbreviation:μSBS, micro shear bond strength)
ca: 21.66±32MPa). The fracture mode in different
groups was studied using a stereo microscope. The
re-sults showed that the fracture mode in all four groups
was adhesive type.
The use of zirconia as a core in dental crowns improves
fixed prosthesis due to high strength, tissue
compatibil-ity, and beauty. However, one of the main
disad-vantages of the Zirconia framework is the low tendency
to react chemically with cement and thereby its weak
bond. Thus, various techniques and materials have been
used for improving the bond between zirconia and resin
cement [1-5]. The aim of the present study was to
inves-tigate the bond strength between zirconia and resin
ce-ment after the preparation of zirconia surface by silica
or aluminosilicate sol-gel dip coating. In this study, the
results showed that the µSBS of the sandblasted
sam-ples and those coated with silica and aluminosilicate by
sol-gel dip coating method was significantly higher than
there is no influence of Y-TZP surface treatment with
sol-gel dip coating on the resin bond strength to Y-TZP
is rejected. In the sol-gel dip coating method, the sol is
first placed on the sample.
Then, the solvent evaporates and nano-silica and
nano-aluminosilicate gels are bonded to the zirconia
surface through Van der Waals electrostatic forces.
Fi-nally, Si-O-Si bonds in silica and Al-O-Si bonds in
alu-minosilicate are reinforced by heat treatment and a solid
layer binds to the surface. Then, hydroxyl groups (a
chemical group with high polarity) in silica or
alumino-silicate coated samples increase the surface polarity and
reactivity of chemical bonds with other chemicals .
This reaction and formation of a new layer on the
zirco-nia surface were confirmed by SEM, EDS, FTIR and
XRD analysis in our previous study .
The self-adhesive luting cement (Clearfil SA,
Ku-rary,Japan) used in this study is an MDP-based silane
containing resin cement. Previous studies showed that
these characteristics have improved the bonding
be-tween resin cement and neutral surfaces like zirconia
and alumina core surface or silica-based surface due to
silanization [31-33]. Therefore, this cement was used
for its high adhesive strength to Y-TZP ceramics. In this
study, micro shear-bond strength of 21.66 MPa was
reported for Clearfil SA after one-day storage in water,
which were significantly higher than those obtained
with the RelyX Unicem (3M ESPE;USA) and Variolink
II (Ivoclar Vivadent, Liechtenstein) composite luting
agents (19.9 and 15.2MPa) [14-15].
One of the common methods used to create
micro-mechanical retention on the surface and increase bond
strength is sandblasting with alumina powder.
Accord-ing to the results, sandblastAccord-ing increases the bond
strength of resin to zirconia. This increase can be due to
micromechanical retention and the bond of hydroxyl
groups of alumina and MDP monomer of resin cement
. Jevinkar P et al.  also used 110-µm alumina
particle for sandblasting and found an increase in the
cement bond strength to zirconia. However,
sandblast-ing with alumina or silica-alumina (Cojet) might
in-crease surface stress making crack formation and
distri-bution during the time [23-25]. Some authors
recom-mended sandblasting with particle size below 50 µm,
applying to sandblast at low pressure (1 to 2 bars) in
order to minimize zirconia surface microcrack .
According to Chen C et al. , cement bond
strength to zirconia in samples coated with nano-silica
by sol-gel method was significantly higher than
sand-blasted samples. However, Lung C et al.  found that
the bond strength of composite resin to zirconia
pre-pared by sandblasting was higher than the samples,
which were coated with silica by using sol-gel method.
The differences observed, can be attributed to the
meth-od used by Lung C et al.  as they used sandblasting
of silica-coated alumina particles.
Various studies show the reasonable performance of
the sol-gel method in creating a layer of nano-silica. In
our study, a silica or aluminosilicate network forms,
through hydrolysis and polycondensation reaction. On
the other hand, existing Si-OH and Al-OH have the
potential to create a chemical bond to resin. As another
advantage, in the sol-gel method, less working space
and cheaper chemicals are used in comparison to
expen-sive machines used for sandblasting.
So far, the silica sol-gel coating technique been used
to increase the bond strength to zirconia. This is the first
study in which aluminosilicate particles are coated on
the surface by a sol-gel dip coating method. According
to literature, the zirconia surface has been mainly coated
with nano-alumina. Külünk T et al.  found no
in-crease in resin bond strength to zirconia coated with a
layer of nano-alumina particles. The reactive magnetron
sputtering method had been used in their study. On the
other hand, Jevincar P et al.  and Zhang et al. 
found an increase in resin bond strength after nano
alu-mina coating by immersing the blocks in the AlN
sus-pension. In this study, aluminosilicate coating improved
the µSBS but this strength is less than sandblast and
silica-coated groups, this is probably due to silica
parti-cles that fill the gaps between alumina partiparti-cles and
inhibit the resin tag formation, which is important in
According to the results of the present study, the use of
nano-silica and aluminosilicate coatings on zirconia can
increase the µSBS of resin cement to zirconia.
There-fore, methods other than a mechanical procedure like
thribochemical coating technique, which may have long
destructive effects on the zirconia- resin cement
The authors thank the Vice Chancellor for Research and
Technology of the Mashhad University of Medical
Sci-ence for funding this study. The current study was
sup-ported by the Vice Chancellor for Research and
Tech-nology, Mashhad University of Medical Science,
Conflict of Interests
Authors declare no conflict of interest.
 Kern M, Wegner SM. Bonding to zirconia ceramic:
ad-hesion methods and their durability. Dent Mater. 1998;
 Chaiyabutr Y, McGowan S, Phillips KM, Kois JC,
Giordano RA. The effect of hydrofluoric acid surface
treatment and bond strength of a zirconia veneering
ce-ramic. J Prosthet Dent. 2008; 100: 194-202.
 Pilo R, Dimitriadi M, Palaghia A, Eliades G. Effect of
tribochemical treatments and silane reactivity on resin
bonding to zirconia. Dent Mater. 2018; 34: 306-316.
 Behr M, Proff P, Kolbeck C, Langrieger S, Kunze J,
Handel G, et al. The bond strength of the
resin-to-zirconia interface using different bonding concepts. J
Mech Behav Biomed Mater. 2011; 4: 2-8.
 Attia A. Bond strength of three luting agents to zirconia
ceramic- influence of surface treatment and
thermocy-cling. J Appl Oral Sci. 2011; 19: 388-395.
 Kitayama S, Nikaido T, Ikeda M, Alireza S, Miura H,
Tagami J. Internal coating of zirconia restoration with
sil-ica-based ceramic improves bonding of resin cement to
dental zirconia ceramic. Biomed Mater Eng. 2010; 20:
 Özcan M, Bernasconi M. Adhesion to zirconia used for
dental restorations: a systematic review and
meta-analysis. J Adhes Dent. 2015; 17: 7-26.
 Thammajaruk P, Inokoshi M, Chong S, Guazzato M.
Bonding of composite cements to zirconia: A systematic
review and meta-analysis of in vitro studies. J Mech
Be-hav Biomed Mater. 2018; 80: 258–268.
 Ikemura K, Tanaka H, Fujii T, Deguchi M, Endo T,
Kadoma Y. Development of a new single-bottle
multi-purpose primer for bonding to dental porcelain, alumina,
zirconia, and dental gold alloy. Dent Mater J. 2011; 30:
Phark JH, Duarte S Jr, Blatz M, Sadan A. An in vitro
evaluation of the long-term resin bond to a new densely
sintered high-purity zirconium-oxide ceramic surface. J
Prosthet Dent. 2009; 101: 29-38.
Derand T, Molin M, Kvam K. Bond strength of
compo-site luting cement to zirconia ceramic surfaces. Dent
Ma-ter. 2005; 21: 1158-1162.
Thompson JY, Stoner BR, Piascik JR, Smith R.
Adhe-sion/cementation to zirconia and other non-silicate
ce-ramics: where are we now? Dent Mater. 2011; 27: 71-82.
Abdalla M, Lung Ch, Tsoi J. Dental Resin-Zirconia
Bonding Promotion Using High-Silica PVD Coating with
High Ionization Sputtering Processing. Coating. 2019; 9:
Chen C, Chen G, Xie H, Dai W, Zhang F. Nanosilica
coating for bonding improvements to zirconia. Int J
Na-nomedicine. 2013; 8: 4053-4062.
Piwowarczyk A, Lauer HC, Sorensen JA. The shear bond
strength between luting cements and zirconia ceramics
after two pre-treatments. Oper Dent. 2005; 30: 382-388.
Jevnikar P, Krnel K, Kocjan A, Funduk N, Kosmac T.
The effect of nano-structured alumina coating on
resin-bond strength to zirconia ceramics. Dent Mater. 2010; 26:
Lung C., Kukk E, Matinlinna JP. The effect of
silica-coating by sol-gel process on resin-zirconia bonding.
Dent Mater J. 2013; 32: 165-172.
Külünk T, Külünk S, Baba S, Oztürk O, Danişman S, Savaş S. The effect of alumina and aluminium nitride
coating by reactive magnetron sputtering on the resin
bond strength to zirconia core. J Adv Prosthodont. 2013;
Queiroz JR, Duarte DA, Fissmer SF, Massi M, Bottino
MA. Deposition of SiOx thin films on Y-TZP by reactive
magnetron sputtering: influence of plasma parameters on
the adhesion properties between Y-TZP and resin cement
for application in dental prosthesis. Mat Res. 2011; 14:
Zhang S, Kocjan A, Lehmann F, Kosmac T, Kern M.
Influence of contamination on resin bond strength to
nano-structured alumina-coated zirconia ceramic. Eur J
Oral Sci. 2010; 118: 396-403.
Lin J, Shinya A, Gomi H, Shinya A. Effect of
self-adhesive resin cement and tribochemical treatment on
bond strength to zirconia. Int J Oral Sci. 2010; 2: 28-34.
Phase transformation of zirconia ceramics by
hydrother-mal degradation. Dent Mater J. 2011; 30: 286-292.
Re D, Augusti D, Augusti G, Giovannetti A. Early bond
strength to low-pressure sandblasted zirconia: evaluation
of a self-adhesive cement. Eur J Esthet Dent. 2012; 7:
Kosmac T, Oblak C, Jevnikar P, Funduk N, Marion L.
The effect of surface grinding and sandblasting on
flex-ural strength and reliability of Y-TZP zirconia ceramic.
Dent Mater. 1999; 15: 426-433.
Wolfart M, Lehmann F, Wolfart S, Kern M. Durability of
the resin bond strength to zirconia ceramic after using
different surface conditioning methods. Dent Mater.
2007; 23: 45-50.
Bielen V, Inokoshi M, Munck JD, Zhang F, Vanmeensel
K, Minakuchi S, et al. Bonding Effectiveness to
Differ-ently Sandblasted Dental Zirconia. J Adhes Dent. 2015;
Madani A, Nakhaei M, Karami P, Rajabzadeh G, Salehi
S, Bagheri H. Sol-gel dip coating of yttria-stabilized
te-tragonal zirconia dental ceramic by aluminosilicate
nano-composite as a novel technique to improve the bonding of
veneering porcelain. Int J Nanomedicine. 2016; 11: 3215-
Catauro M, Bollino F, Papale F, Gallicchio M, Pacifico
S. Influence of the polymer amount on bioactivity and
biocompatibility of SiO2/PEG hybrid materials
synthe-sized by sol-gel technique. Mater Sci Eng C Mater Biol
Appl. 2015; 48: 548-55.
Cao Y, Dai WL, Deng JF. The synthesis, characterization
and application of Ag–SiO 2–Al 2O3 sol-gel composites.
Materials Lett. 2001; 50: 12-7.
Fardad MA. Catalysts and the structure of SiO2 sol–gel ﬁlms. J Mater Sci. 2000; 35: 1835–1841.
Donassollo TA, Demarco FF, Della Bona A. Resin bond
strength to a zirconia-reinforced ceramic after different
surface treatments. Gen Dent. 2009; 57: 374-379.
Matinlinna JP, Vallittu PK. Bonding of resin composites
to etchable ceramic surfaces- an insight review of the
chemical aspects on surface conditioning. J Oral Rehabil.
2007; 34: 622-630.
Inokoshi M, Kameyama A, De Munck J, Minakuchi S,
Van Meerbeek B. Durable bonding to mechanically
and/or chemically pre-treated dental zirconia. J Dent.